Parameters based on the hardness and elastic moduli, used as indicators of abrasion resistance and their physical meanings
Modeling the wear rate is a complex process. The several possibilities of chemical, physical and mechanical changes at the interface are the most probable reasons for this . In this manner, it is reasonable to consider the wear rate as a stochastic process [2, 3], and indeed this approach was taken into account by Archard , when he formulated his well-known model. Since then, the majority of available models are based on his proposition, independent on the characteristics of mechanical system. Considering a sharp contact, both Torrance  and Yi-Ling & Zi-Shan  for sliding and rolling abrasion, respectively, modified Archard’s equation based on elastic effects, and the ratio of the hardness (H) to the Young’s modulus (E) was the main parameter of the models. In a tribological system with dissimilar materials, for example a ceramic abrading a metal, one material can experience the yielding and the other the brittle failure. This difference in the mechanical behaviors can be decisive for the final performance to wear.
The use of Young’s modulus to model the wear resistance was applied for coatings ; it appeared in other modifications of Archard’s equation , and even in empirical relationships between the wear rate and the mechanical properties . Eventually, in all cited cases, the elastic modulus was not the reduced one (Er), as will be treated here.
A selection of parameters involving hardness and elastic moduli can be summarized (Table 1) [9-11]. All of them have physical meanings that possess some interest for abrasion resistance of materials. The last parameter presented in Table 1, H3/E2, is proportional to the load that defines the transition between elastic to plastic contact in a ball-on-plane system, applying the analytical solutions provided by Hertz in Contact Mechanics , where the reduced modulus is already taken into account.
|H/E||Deformation relative to yielding |
|(H/E)2||Transition on mechanical contact – elastic to plastic |
|H2/2E||Modulus of resilience |
|H/Er 2||Resistance to the plastic indentation |
|H3/E2||Resistance to the plastic indentation |
Using some of the abovementioned solutions, a case study will be presented. For two tribological pairs with known wear coefficients, the ratio of hardness to reduced modulus works well than the single property of the worn material (E). The expectation regarding the H/Er ratio is confirmed also by other aspects used to characterize abrasion, especially the cutting efficiency.
2. Modelling abrasion with E/H ratio
In 1980 Torrance  published a model for abrasive wear rate based on the elastic recovery after scratching, supposing that the abrasive particle has a conical geometry. This choice is suitable, because there is an analytical model to describe the changes at the recovered surface . Some years later, another paper  adopted the same physical basis but here the application occurred to systems where the abrasive particles roll, instead of slide. The key similarities and differences of both manuscripts will be discussed below.
First of all, it is important to see the main definition presented in , because it was the basis for the referred models. This reference presents an equation that relates the reduced modulus with the amount of elastic recovery, he (indicated in Figure 1), considering a conical indenter:
In Equation 1 the term Er is the reduced modulus, defined as:
Er is the reduced modulus;
Ei is the Young’s modulus of conical indenter;
νi is the Poisson’s ratio of conical indenter;
E is the Young’s modulus of tested material, and;
ν is the Poisson’s ratio of tested material.
A modern definition for the term E/(1-ν2) can be found in ISO/FDIS 14577-1 standard , and it is called as ‘indentation modulus’, using the symbol EIT. Exactly this term was used by references  and . In this way, the mechanical properties of abrasive particle were discarded in both cases. It is notable that this aspect has not been ruled out by Stilwell and Tabor  in 1961.
A great difference between the Torrance’s paper  and the Yi-Ling and Zi-Shan one  is with respect to the volume of wear. In the former, it was taken as directly proportional to h2, and for the latter, related to hP2, following the symbology of Figure 1. The latter can be considered as more appropriate because it takes into account the elastic effects at a worn surface, so that the final formulation provided by  will be presented. Thus, an equation for wear rate, Q (m3/m), can be written as:
W is the applied load;
H is the hardness of worn material;
C is a constant and;
KP will be called here as partial wear coefficient, based on elastic effects during indentation, defined as , being k another constant.
In order to differentiate the use of elastic modulus to the reduced one, another symbology will be considered for the latter case, where KP’ is introduced:
k is a constant.
To define the constant C, Yi-Ling and Zi-Shan  made use of nine constants to fit the experimental results. The constant k of term KP varies with many variables of tribosystem. On the other hand, although Torrance  has not make use of constants to fit experimental results obtained by others [15-17], he chose a material as reference (a steel of 401 HV hardness), and all cases were then compared with this material (Equation 5). In this way, he only needed to calculate the constant k (=10), finding a very interesting result, as can be seen in Figure 2.
Figure 2 shows a linear relationship between the relative wear resistance βi and the relative partial wear coefficient, defined in  as βi* (Equation 5). The experimental points used to build this curve included pure metals and heat-treated steels. These groups of materials do not present the same behavior when they are abraded by hard particles (Figure 3).
In other words, a pure metal with similar hardness of heat-treated steel presents a higher abrasion resistance. This implies that steels present a different slope on a wear resistance curve when it is put as a function of hardness. Using the ratio of the hardness to the Young’s modulus, Torrance  put in the same curve these referred groups of materials, which present, a priori, different behaviors. This kind of result was also described in reference , but based on a different approach. This research made use of the abrasion factor (fab) definition (Equation 6 and Figure 4 ) to describe the wear resistance. It is a parameter related with the cutting efficiency, i.e., when this factor is equal to unity only the micro-cutting would be the wear mechanism, while for values correspondent to zero no removal of material would be detected. The experimental results obtained in  are shown in Figure 5.
A1 is the cross section area relative to pileup produced by a single scratch and;
A2 is the cross section area relative to the groove produced by a single scratch.
Again, in Figure 5 both pure metals and steels are put in the same curve, showing that the hardness alone, in some cases, is not a complete descriptor of the wear resistance. The similarity between the results presented in Figure 2 and Figure 5 opens a possibility to the abrasion factor to be described as a function of the hardness-to-elastic modulus ratio.
Although in reference  the elastic effects have not been incorporated to the model, there are results in the literature relating the pileup formation (Figure 6, ) with the mechanical properties . In this case, it is possible to consider that the pileup formation (hc/h) works for static (hardness test) and kinetic cases (scratch test), being the higher the pileup, the smaller the cutting efficiency.
3. Case study
Two tribological pairs were studied, also considered in a previous investigation . Their wear rates are known: glass abrading a quenched and tempered (Q&T) 52100 steel , and alumina wearing a hard metal . The mechanical properties, determined from instrumented indentation testing, used to calculate the partial wear coefficients, KP and KP’ (Equations 3 and 4), are presented in Table 2. To calculate the reduced modulus (Equation 2), Poisson’s ratios were extracted from .
As seen in the previous item, due to the similarity of Figures 2 and 5, the partial wear coefficient can be well related to the abrasion factor (cutting efficiency), fab. An indirect way to know the fab factor is found in reference , which defined it as the ratio between the wear coefficient K (Archard’s definition) and the ploughing fraction of friction coefficient (μp). The cutting efficiency values, following this definition, are 0.106 for glass abrading bearing steel and 0.079 for alumina wearing hard metal, a difference of 34%. As the constant KP’ can vary along a broad range (Figure 8), we select a value so as to the difference is also 34%, and for this purpose it is 8.25.
|Hard metal (grade K)||11||480||0.023||0.049|
An example of variation in KP’ value with k factor is presented in Figure 8, for the tribological pairs considered in Table 2. Another pair was added (calcite-fluorite) in this figure, in order to help the discussion with their differences.
The resulting values of partial wear coefficients, using 8.25 as k factor, are presented in Table 3.
|Glass - Q&T steel||1.41||2.66|
|Alumina – Hard metal||1.41||1.98|
Table 3 shows that the KP values were similar for the studied pairs, while the KP’ did not follow this trend. The wear coefficients of tribological pairs (K values) determined using sliding abrasion tests were 0.014 and 0.008, for glass against steel  and alumina against hard metal , respectively. Visibly this difference in wear rates is only reflected by the KP’ values, which is a direct result of the ratio of hardness to the reduced modulus.
Another observation for the KP values is that the similarity presented in Table 3 is not affected by the variation of the k factor. On the contrary, KP’ is strongly dependent on this factor, as can be seen in Figure 8.
One can ask about the good agreement with experimental data found in  and  when they used only the Young’s modulus in wear model. The key point for that is the superiority of abrasive hardness in relation to the worn surface. All experimental results in these cases were performed using abrasives much harder than the tested materials, such that the mechanical properties of them can be considered as unaltered along the tests. An investigation  showed significant changes in glass particles when they abraded steel surfaces, even for non heat-treated ones. The same thing was demonstrated in  for different abrasives wearing WC-Co thermal sprayed coatings. When the abrasive particle is relatively soft to the abraded material, their mechanical properties play a key role during the wear process, and an extensive discussion on it can be found in .
In addition, in reference  these tribological pairs were separated using the difference in the plasticity index, δH, defined in  (Equation 8), being the smallest difference related to the calcite-fluorite, and the largest for glass-steel pair within the materials analyzed in . This aspect seems to be important again when one observes Figure 8. When the difference is insignificant, as in the case of calcite-fluorite, the variation of KP’ with k factor is minor, and on the other hand, for the case of the glass-steel pair, for a notable difference in the plasticity index, a great variation of KP’ with the k factor occurs.
A brief discussion of the k factor is instructive. Following , this factor is especially associated to the particle geometry. As stated, a hypothetical KP’ of calcite-fluorite pair would be less affected by the variation on k factor. Therefore, one can imagine a small fragment of mineral used in Mohs scale  and, considering the previous assertive, conclude that its geometry would not be important. Probably, this is not the case. The k factor should be understood in a broad manner, i.e., all variables of a system can alter its value. Thus, slight changes in tribological variables could bring higher alterations in the wear coefficient for the pair glass-steel than for the other described cases. At this moment, no experimental result is available to corroborate this hypothesis, but it is an interesting field to be explored further.
Finally, a discussion concerning the Equation (7) and the values presented in Table 2 is valuable. If the values of H/E ratio for steel and alumina were applied in Equation (7), the results would be similar. A similar height of pileup for these materials obviously is not a reasonable result, taking into account the experimental values obtained for wear and friction coefficients for them. Nevertheless, applying the reduced modulus in the place of E in that equation, one can find fewer tendencies to form pileup after abrasion of steel by glass, which means a higher cutting efficiency in this case, meeting with the values described before. Consequently, it is more a case of successful application of reduced modulus to predict changes at the mechanical contact.
4. Conclusions and final remarks
The viability of the use the hardness-to-reduced modulus ratio to model the wear coefficient for abraded materials was demonstrated. Previous models were developed taking into account only the Young’s modulus of worn surface, discarding the properties of abrasive material. These cases work only for pairs where the abrasive particle is harder than the abraded material and it was demonstrated that they fail when the abrasive hardness is relatively low.
In addition, other questions were discussed and they open some possibilities to carry out future research. First, the model of wear coefficient treated here involves higher requirements, because a constant is needed. This constant seems to affect more the wear coefficient of some pairs than the others, and the reason for that is not clear. Finally, an extensive work could be made exploring the relation between cutting efficiency (abrasion factor) and H/Er ratio, computing a large variation of the applied load and the abrasive (indenter) properties. Probably, an investigation based on these aspects should supply answers to the improvement of a wear model containing the H/Er ratio.
Financial support for this study was provided by CNPq under project no. 306727/2011-0.
A1 and A2 Cross section areas used in the definition of abrasion factor
E Young’s modulus
Ei Young’s modulus of indenter
Er Reduced modulus
Young’s modulus of a reference material
fab Abrasion factor or cutting efficiency
Vickers hardness of the worn material
Vickers hardness of wear debris
Vickers hardness of a reference material
h Maximum depth at applied load
hC Contact depth
he Elastic recovery
hP Final depth
hS Deflected depth
K Wear coefficient
KP Partial wear coefficient, defined as
KP’ Partial wear coefficient calculated with Er instead of E
Q Wear rate
Q’ Wear resistance (= 1/Q)
W Applied load
βi Relative wear resistance
βi* Relative partial wear coefficient
μp Ploughing fraction of friction coefficient, taken as 0.2
ν Poisson’s ratio of the worn material
νi Poisson’s ratio of the indenter
Bayer R.G., Comments on Engineering Needs and Wear Models. In: Ludema K.C., Bayer, R.G. (eds.) Tribological Modeling for Mechanical designers. Philadelphia: ASTM International; 1991. p. 3-11.
Silva Jr., C.R.A., Pintaude G., Al-Qureshi H. A., Krajnc M.A. An Application of Mean Square Calculus to Sliding Wear. Journal of Applied Mechanics 2010;77(2) paper 021013.
Silva Jr., C.R.A., Pintaude G. Uncertainty Analysis on the Wear Coefficient of Archard Model. Tribology International 2008;41(6) 473-481.
Archard J.F. Contact and Rubbing of Flat Surfaces. Journal of Applied Physics 1953;24(8) 981–988.
Torrance A.A. The Correlation of Abrasive Wear Tests. Wear 1980;63(2) 359-370.
Yi-Ling W., Zi-Shan W. An Analysis of the Influence of Plastic Indentation on Three-Body Abrasive Wear of Metals. Wear 1988; 122(2) 123-133.
Leyland A., Matthews A. On the Significance of the H/E Ratio in Wear Control: a Nanocomposite Coating Approach to Optimised Tribological Behaviour. Wear 2000; 246(1-2) 1-11.
Liu R., Li D.Y. Modification of Archard’s Equation by Taking Account of elastic/pseudoelastic Properties of Materials. Wear 2001; 251(1-12) 956-964.
Finkin E.F. Examination of abrasion Resistance Criteria for Some Ductile Metals. Journal of Lubrication Technology 1974;96(2) 210-214.
Joslin D.L., Oliver W.C. A New Method for Analyzing Data from Continuous Depth-Sensing Microindentation Tests. Journal of Materials Research 1990; 5(1) 123-126.
Tsui T.Y., Pharr G.M., Oliver, W.C., Bhatia C.S., White R.L., Anders A., Brown I.G. Nanoindentation and Nanoscratching of Hard Carbon Coatings for Magnetic Disks. MRS Proceedings 1994;356, p.767.
Brizmer V., Kligerman Y., Etsion I. The Effect of Contact Conditions and Material Properties on the Elasticity Terminus of a Spherical Contact. International Journal of Solids and Structures 2006; 43(18-19) 5736–5749.
Stilwell, N. A., Tabor, D. Elastic Recovery of Conical Indentations. Proceedings of the Physical Society 1961; 78(2) 169-179.
ISO - International Organization for Standardization. ISO/FDIS 14577-1 - Metallic Materials - Instrumented Indentation Test for Hardness and Material Parameter - Part 1: Test method. Geneva, Switzerland, 2002.
Richardson R.C.D. The Maximum Hardness of Strained Surfaces and the Abrasive Wear of Metals and Alloys, Wear, 1967; 10(5) 353-382.
Richardson R. C. D. The Wear of Metals by Hard Abrasives, Wear 1967; 10(4) 291-309.
Richardson R.C.D. The Wear of Metals by Relatively Soft Abrasives, Wear 1968; 11(4) 245-275.
Murray M.J., Mutton P.J., Watson J.D. Abrasive Wear Mechanisms in Steels. In: Ludema K.C., Glaeser W.A., Rhee S.K. (eds.), WOM 1979: Proceedings of International Conference on Wear of Materials, 16-18 April 1979, Dearborn, MI. New York: American Society of Mechanical Engineers, pp. 257–265, 1979.
Zum Gahr, K.H. Modelling of Two-Body Abrasive Wear. Wear 1987; 124(1) 87–103.
Buttery T.C., Archard J.F. Grinding and abrasive wear. Proceedings of the Institution of Mechanical Engineers 1970; 185(1) 537-552.
Pintaude G., Hoechele A.R., Cipriano G.L. Relation between Strain Hardening Exponent of Metals and Residual Profiles of Deep Spherical Indentation. Materials Science and Technology 2012; 28(9-10) 1051-1054.
Jardret V., Zahouani H., Loubet J.L., Mathia T.G. Understanding and Quantification of Elastic and Plastic Deformation during a Scratch Test. Wear 1998; 218(1) 8-14.
Masen M.A., de Rooij M.B., Schipper D.J., Adachi K., Kato K. Single asperity abrasion of coated nodular cast iron. Tribology International 2007; 40(2)170–179.
Pintaude G. An Overview of the Hardness Differential Required for Abrasion, Journal of Tribology 2010;132(3) paper 034502.
Pintaude G., Bernardes F.G., Santos M.M., Sinatora A., Albertin E. Mild and Severe Wear of Steels and Cast Irons in Sliding Abrasion. Wear 2009;267(1-4) 19-25.
Pintaude G., Farias M.C.M., Kohnlein M., Tanaka D.K., Sinatora A. Abrasive Wear of Cutting Tools Used in the Wood Industry (In Portuguese). In: UFRN – Universidade Federal do Rio Grande do Norte (ed.) CONEM 2000: XV Brazilian Congress of Mechanical Engineering, 7-11 August 2000, Natal, Brazil. Rio de Janeiro: Associação Brasileira de Ciências Mecânicas, 2000.
Gercek H. Poisson’s Ratio Values for Rocks. International Journal Rock Mechanics and Mining Sciences 2007;44(1) 1–13.
Jacobson S., Wallen P., Hogmark S. Fundamental Aspects of Abrasive Wear Studied by a New Numerical Simulation Model. Wear 1998;123(2) 207-223.
Pintaude G., Tanaka D.K., Sinatora A. The Effects of Abrasive Particle Size on the Sliding Friction Coefficient of Steel using a Spiral Pin-on-Disk Apparatus. Wear 2003; 255 (1-6) 55-59.
Bozzi A. C.; De Mello J.D.B. Wear Resistance and Wear Mechanisms of WC-12%Co Thermal Sprayed Coatings in Three-Body Abrasion, Wear 1999;233-235, 575-587.
Pintaude, G. (2011). Characteristics of Abrasive Particles and Their Implications on Wear, New Tribological Ways, Ghrib, T. (Ed.), ISBN: 978-953-307-206-7, InTech, Available from: http://www.intechopen.com/books/new-tribological-ways/characteristics-of-abrasive-particles-and-their-implications-on-wear
Milman Y.V., Galanov B.A., Chugunova B.I. Plasticity Characteristic Obtained through Hardness Measurement, Acta Metallurgica et Materialia 1993; 41(9) 2523-2532.
Broz M.E., Cook R.F., Whitney D.L. Microhardness, Toughness, and Modulus of Mohs Scale Minerals. American Mineralogist 2006; 91(1) 135–142.